Ilmenite-type structure and pervoskite structure mix-phase ceramics at microwave frequency

ABSTRACT The impact of CuB2O4 additive used as a sintering aid on the microstructures and microwave dielectric characteristics of mixed phase (Mg0.95Zn0.05)Co0.05TiO3-Ca0.6(La0.9Y0.1)0.2667TiO3 ceramics was investigated. CuB2O4 additives can effectively lower the densification temperature of (Mg0.95Zn0.05)Co0.05TiO3-Ca0.6(La0.9Y0.1)0.2667TiO3 from 1450°C to the range of 1050°C ~ 1175°C. Doping CuB2O4 (0.25 ~ 2 wt%) in 0.875(Mg0.95Zn0.05)Co0.05TiO3-0.125Ca0.6(La0.9Y0.1)0.2667TiO3 ceramics can substantially enhance their microwave dielectric properties and density. With the addition of 1% and 0.25% CuB2O4, Q × f values of 43,000 GHz and 7700 GHz were obtained at 1050–1175°C, respectively. Different additions of CuB2O4 have a significant effect on the Q × f value. Temperature coefficient of resonant frequency of 0.875(Mg0.95Zn0.05)Co0.05TiO3-0.125Ca0.6(La0.9Y0.1)0.2667TiO3 (0.875MZCT–0.125CLYT) varied from 16 to 30.9 ppm/°C when adding different CuB2O4 (0.25 ~ 2 wt%).


Introduction
As mobile communication technology enters the (5th generation mobile networks) 5 G era, the development of massive multi-input multi-output (MIMO) technology, coupled with the increasingly stringent requirements brought by base station integration, puts forward higher requirements for filters [1,2].Microwave ceramic filter element media, which has received a lot of interest in the field of nextgeneration filters [2,3], has a comprehensive advantage of light weight and good temperature drift resistance under the premise of achieving the core performance requirements [4][5][6][7][8].
The manufacture of powder raw materials and the improvement of ceramic properties of microwave dielectric are now the most challenging technical issues to overcome in order to better fulfill the development needs of ceramic filters.Permittivity(ε r ), quality factor (Q × f), and temperature coefficient of resonant frequency are the three main characteristics of microwave dielectrics.A low ε r can shorten the signal transmission time, a high Q × f can increase the selectivity and longevity of microwave components, and a temperature coefficient of resonant frequency close to zero can allow electronic devices to operate reliably in a range of temperature environments [9][10][11][12][13][14][15][16][17][18].
MgTiO 3 -based microwave dielectrics have been intensively studied for years with low dielectric loss.MgTiO 3 -CaTiO 3 ceramics made of a mixture of modified magnesium titanate and perovskite structured calcium titanate have been applied in dielectric resonators and patch antennas.With a ratio of Mg:Ca = 95:5, 0.95 MgTiO 3 -0.05CaTiO 3 mixed phase ceramic has an ε r ~21, a Q×f ~ 56,000 (at 7 GHz), and a zero τ f value [19].With the partial replacement (Mg 0.7 Zn 0.3 ) by Co, (Mg 0.7 Zn 0.3 ) 0.95 Co 0.05 TiO 3 had excellent dielectric properties with an ε r ~20, Q×f ~ 163,560 GHz, and a τ f ~ −65 ppm/ o C. To produce a temperature-stable material, Ca 0.6 (La 0.9 Y 0.1 ) 0.2667 TiO 3 which has a large positive τ f value of +380 ppm/ o C, was added to (Mg 0.7 Zn 0.3 ) 0.95 Co 0.05 TiO 3 .
There are three approaches to reducing the sintering temperature of microwave dielectric ceramics: low melting sintering aids addition [20][21][22], chemical processing, and the use of smaller particles as the starting materials.Of these three, sintering aids addition is the most effective and least expensive.However, no liquid-phase sintering of xMZCT-(1-x)CLYT with sintering aids addition has been reported yet.Previously, CuB 2 O 4 was researched and found to have good dielectric properties [23].
In this paper, CuB 2 O 4 was used as a sintering aid for reducing the sintering temperature of xMZCT-(1-x)CLYT ceramics.The effects of CB content on the densification, phase development and dielectric properties of 0.875MZCT-0.125CLYTceramics are investigated.The analysis focused on the crystal phase, microstructure, and microwave dielectric properties of 0.875MZCT-0.125CLYTceramics intermixed with CuB 2 O 4 .

Experimental
Samples for the 0.875MZCT-0.125CLYTwere created using traditional solid-state techniques.The initial components are combined in accordance with the stoichiometric ratio.For CuB 2 O 4 powder, high-purity powders of CuO and H 3 BO 3 were weighed, mixed and calcined at 850°C for 3 h.As a sintering aid, a trace amount of CuB 2 O 4 (0.25%-2% weight) was used.The (Mg 0.95 Zn 0.05 )Co 0.05 TiO 3 were synthesized using a solid-state mixed oxide route with starting materials of high-purity oxide powders (>99.9%):MgO, ZnO, CoO and TiO 2 .Because MgO is hygroscopic, it was first fired at 600°C to avoid moisture contain.The weighed raw materials were mixed by ball milling with agate media in distilled water for 24 h, and the mixtures were dried and calcined at 1100°C for 4 h.Samples of Ca 0.6 (La 0.9 Y 0.1 ) 0.2667 TiO 3 ceramics were processed using a conventional solid-state reaction from high-purity oxide powders (CaCO 3 , La 2 O 3 , Y 2 O 3 , and TiO 2 ).After mixing, milling for 24 h, drying, and grinding, the mixtures were calcined at 1000 •C for 2 h.
The powder calcination at different temperatures, then mix with massage fraction 0.875MZCT-0.125CLYT.The calcined powder was mixed with varying quantities of CuB 2 O 4 additives serving as sintering aids to achieve the desired composition of 0.875MZCT-0.125CLYT.It was subsequently reground with Polyvinyl alcohol (PVA) solution as a binder for 5 h.Uniaxial pressing is used to press particles having a 1.1 cm diameter and 0.5 cm thickness.At 120 MPA, all samples were compressed.These particles are sintered in air for hours at a temperature between 1050 and 1175°C after being degreased.
X-ray diffraction (XRD) with CuK α1 radiation (XRD-7000, Shimadzu, Kyoto, Japan) was used to examine the phase purity and crystal structure of 0.875MZCT-0.125CLYTceramics.The Archimedes method was used to calculate the bulk densities.
Using a scanning electron microscope (FE-SEM, Model S4800; Hitachi, Japan), microstructure images were taken.The Agilent E8362B network analyzer was used to measure the permittivity and quality factor values in the TE011 mode, following the Hakki-Coleman method [24,25].The temperature coefficient of resonant frequency (τ f ) was measured for a temperature range of 25-85°C to determine the temperature coefficient of resonant frequency.The following equation was used to determine the value of τ f : Where f1 denotes the resonant frequency at T1 and f2 denotes the resonant frequency at T2. that the average ion radii of Ca 2+ , La 3+ , and Y 3+ were bigger than those of Mg 2+ (72 pm) the solid solution could not be produced.MgTi 2 O 5 usually formed as an intermediate phase.According to the XRD patterns, the (Mg 0.95 Zn 0.05 )Co 0.05 TiO 3 phase exists in these specimens.X-ray diffraction patterns of 0.875MZCT-0.125CLYTceramics system have not been changed significantly with sintering temperatures in the range 1050-1175°C.The XRD patterns show peaks indicating the presence of (Mg 0.95 Zn 0.05 )Co 0.05 TiO 3 as the main crystalline phase, a minor phase of Ca 0.6 (La 0.9 Y 0.1 ) 0.2667 TiO 3 .Figure 2 displays sintered at various temperatures for 4 h.Four SEM images of 0.875MZCT-0.125CLYTceramics that include CuB 2 O 4 additions of 1 weight percent.As the sintering temperature increased, it was evident that the grain size also increased for the 0.875MZCT-0.125CLYTceramics.However,when 1 wt% CuB 2 O 4 was added, the ceramics did not achieve high density and no grain growth was observed at 1050°C, as indicated by SEM results for different temperatures.As shown in Figure 2, the liquid-phase effect caused an increase in grain size as the sintering temperature.CuB 2 O 4 impact on the liquid phase could be significant.At 1100°C, significant grain development was seen, and for specimens sintered at 1125°C, the holes were virtually completely obliterated.

Results and discussion
Figure 3 depicts the densities of 0.875MZCT-0.125CLYTceramics doped with varying quantities of CuB 2 O 4 throughout a 4-h period at varied sintering temperatures.As shown in the figure, due to the increase in grain size, the density increases to 1 wt% with the increase of sintering temperature and the increase of CuB 2 O 4 additives.The rise in bulk density with a higher sintering temperature may be attributed to the reduction in pore numbers, as depicted in Figure 2, whereas the reduction in bulk density could arise from a typical grain growth.Even with so much CuB 2 O 4 doping, it seems like the bulk density has reached saturation at 1100°C.The maximum density of 0.875MZCT-0.125CLYTwith 1 wt% CuB 2 O 4 is 4.3 g/cm [3] sintered at 1100°C for 4 h.Therefore, the inclusion of CuB 2 O 4 additives can significantly lower the sintering temperature required for 0.875MZCT-0.125CLYTceramics sintering temperature in the CuB 2 O 4 -doped 0.875MZCT-0.125CLYTceramic.Excessive will reduce the density because CB is a glass phase and the CB density is lower than 0.875MZCT-0.125CLYT,and excessive CB addition over 2 wt.% will reduce the density.
When the sintering temperature rises, the energy rises meaning that the grain boundary moves better and it is easy for the small grains to dissolve, so that the grain growth is more uniform and the pores decrease with the increase in the sintering temperature, and densification occurs.In addition, when various additives are added to the 0.875MZCT-0.125CLYTceramics to form liquid-phase sintering, this is more conducive to small-grain dissolution, an increase in the wetting boundary movement rate, and grain rearrangement to achieve densification.This can be compared with the SEM in Figure 2 for the 0.875MZCT-0.125CLYTceramics with multiple sintering aids CB that were sintered at 1050°C for 4 h, where the grains were smaller, more pores appeared, and the density was lower; when the sintering temperature rose to 1100°C, the grain size was consistent, there were fewer pores, and the density was higher.It can be concluded that liquid-phase sintering occurs when using different additives, and when the additive exceeds 2 wt%, it will cause a slight decrease in the density.Generally, in cases of liquid-phase sintering, using appropriate amounts of sintering aids can effectively improve the phaseforming capacity and reduce the sintering temperature.However, when the sintering aid content is excessive, the grains grow excessively, and with a larger particle size, the rearrangement will be subject to greater resistance and there will be a small number of pores in the boundary, meaning it is not easy to discharge and other factors will affect the change in the density and radio-frequency dielectric performances.
The dielectric constant marginally rises as the sintering temperature rises.Additionally, larger CuB 2 O 4 concentration raises the density value, which translates to higher ε r as shown in Figure 4.
Lichterecker [26] proposed an intermediate form between the serial and parallel mixing rules form called logarithmic mixing rule (in the case where α → 0) [26]: where ε h and ε l are the relative dielectric constants of the high-dielectric phase and low-dielectric phase, respectively, V h and V l the volume fractions of the high dielectric phase and low-dielectric phase (V h +V l = 1), ε m the effective dielectric constant of the composite, and α a parameter that determines the type of mixing rule.
The addition of 1 wt% CuB 2 O 4 to the 0.875MZCT-0.125CLYTceramic, accompanied by a rise in sintering temperature from 1050°C to 1100°C, resulted in an increase of ε r value from 26.73 to 28.9.Microwave dielectric loss is influenced by various factors, which can be classified into intrinsic and extrinsic losses.The lattice vibration mode is the primary cause of intrinsic loss, whereas second phase, oxygen vacancy, grain size, and densification or porosity are the main contributors to extrinsic loss [27].It is believed that porous materials are significantly influenced by interfacial polarization [28].
The quality factor (Q × f) value of 0.875MZCT-0.125CLYTceramics that incorporate different CuB 2 O 4 additives at varying sintering temperatures is presented in Figure 5.
Internal factors, such as lattice vibration mode, impact the Q × f value of microwave loss.The presence of cation ordering can often result in an increase in Q × f, thus its absence may frequently lead to a decrease in Q × f [29].
The decrease of Q × f in mixed systems has been associated by some with the loss of cation ordering in ordered cation compounds [30].
However, it should be noted that the reduction of the Q × f value can be due to either intrinsic (i.e.attice    related) or extrinsic mechanisms.At microwave frequencies, the unloaded quality factor is said to be dependent on extrinsic factors like secondary phases, density, and oxygen vacancies.The Q × f value increases to its maximum value and subsequently decreases as the sintering temperature rises.At 1100°C, the maximum Q × f value of 0.875MZCT-0.125CLYTceramic containing 1 wt% CuB 2 O 4 additive is 43,000 GHz.Abnormal grain growth at higher sintering temperatures is responsible for the degradation of the Q × f value, as demonstrated.Conversely, due to the enhancement in densification of the specimen by the liquid phase, CuB 2 O 4 -doped 0.875MZCT-0.125CLYTexhibits a single maximum Q × f value at lower sintering temperatures.Dielectric losses in microwave materials are primarily due to lattice vibration patterns, as well as pores, impurities, second phases, or lattice defects.The controlling role of relative density in these losses has been demonstrated in other types of microwave dielectric materials as well [31,32].
Due to the addition of sintering aids, the Q × f values of the samples in this work are approximately half of those of the samples sintered at 1450°C.However, adding sintering aids can reduce the sintering temperature.
Figure 6 displays the temperature coefficients of resonant frequency (τ f ) for 0.875MZCT-0.125CLYTceramics with different CuB 2 O 4 additives and sintering temperatures.The relationship between the temperature coefficient of resonant frequency (TCF) and the temperature coefficient of dielectric constant (TCK) as well as the thermal expansion coefficient (a) is stated in Equation 4 [33] The linear thermal expansion coefficient, denoted as L, is a constant in ceramics and directly affects the temperature coefficient of capacitance (TCF) through its relationship with TCK.The temperature dependence of the dielectric constant (TCK) can be expressed as three terms(A, B, and C) in Equation (4) [34]: Where and V denote the polariz ability and volume, respectively.The term A (commonly negative) represents the direct dependence of the polarizability on temperature.B and C represent the increase of the polarizability and the decrease of the number of polarizable ions in the unit-cell, respectively; the unit cell volume increased with an increase in temperature.The B and C terms are normally the largest ones but have similar value with opposite signs.Hence, (B+C) has a small positive value.TCK is increased by an increase of the tilting of oxygen octahedra in the perovskite structure, which correspond to a decrease of TCF by Equation ( 4).
The temperature coefficient of the resonant frequency (τ f ) is typically determined by the composition and phase within the ceramic, while demonstrating insensitivity across all sintering temperature ranges.With the increase of CuB 2 O 4 additives, the τ f value becomes more positive.As the sintering temperature varies, the CuB 2 O 4 additive increases from 0.25 wt% to 2 wt% resulting in a variation of 17.5 to 30.9 ppm/ o C. Increasing the amount of CLYT can result in achieving zero τ f , as the τ f values for (Mg 0.95 Zn 0.05 )Co 0.05 TiO 3 and CLYT are −50 and + 310 ppm/ o C, respectively.
The temperature coefficient of resonant frequency (τ f ) for ceramics was related to composition and existing phases.Regardless of sintering temperature range, τ f was not affected.When CuB 2 O 4 additives were increased, the τ f value became more positive and ranged from 17.5 to 30.9 ppm/oC.Increasing CLYT content could achieve zero τ f since (Mg 0.95 Zn 0.05 )Co 0.05 TiO 3 and CLYT had different τf values of −50 and +310 ppm/ o C, respectively.

Conclusion
The study focused on the dielectric properties of 0.875MZCT-0.125CLYTceramics containing CuB 2 O 4 .Secondary phases such as MgTi 2 O 5 were mixed with 0.875MZCT-0.125CLYTceramics, with MgTi 2 O 5 serving as the primary phase.The addition of CuB 2 O 4 in 0.875MZCT-0.125CLYTceramics not only lowers the sintering temperature effectively but also enhances its microwave dielectric properties.At a temperature of 1100°C, ceramics with a composition of 0.875MZCT-0.125CLYTand an addition of 1 wt% CuB 2 O 4 exhibit exceptional microwave dielectric characteristics including εr of approximately 28.9, Q × f value of approximately 43,000 (at 8 GHz), and τ f value of approximately 27.6 ppm/ o C.

Figure 3 .
Figure 3. Bulk density curves were generated for 0.875MZCT-0.125CLYTceramics with varying amounts of CuB 2 O 4 additives sintered at different temperatures for four hours.

Figure 4 .
Figure 4.The dielectric constant curves for 0.875MZCT-0.125CLYTceramics with different amounts of CuB 2 O 4 additives at various sintering temperatures were recorded over a period of four hours.

Figure 5 .
Figure 5.The quality factor values were measured for 0.875MZCT-0.125CLYTsystems with varying amounts of CuB 2 O 4 additives, sintered at different temperatures for four hours.

Figure 6 .
Figure 6.The resonant frequency values of 0.875MZCT-0.125CLYTsystem, with various CuB 2 O 4 additives sintered for four hours at different temperatures, were analyzed for their temperature coefficients.